- About this Journal
- Abstracting and Indexing
- Aims and Scope
- Annual Issues
- Article Processing Charges
- Articles in Press
- Author Guidelines
- Bibliographic Information
- Citations to this Journal
- Contact Information
- Editorial Board
- Editorial Workflow
- Free eTOC Alerts
- Publication Ethics
- Reviewers Acknowledgment
- Submit a Manuscript
- Subscription Information
- Table of Contents
Advances in Mechanical Engineering
Volume 2013 (2013), Article ID 848973, 11 pages
The Experimental Analysis of Forming and Strength of Clinch Riveting Sheet Metal Joint Made of Different Materials
1Faculty of Mechanical Engineering and Aeronautics, Rzeszow University of Technology, al. Powstańców Warszawy 8, 35-959 Rzeszów, Poland
2Faculty of Mechanical Engineering, Technical University of Košice, Mäsiarska 74, 040 01 Košice, Slovakia
Received 19 June 2013; Revised 18 September 2013; Accepted 3 October 2013
Academic Editor: Gang Wang
Copyright © 2013 Jacek Mucha et al. This is an open access article distributed under the Creative Commons Attribution License, which permits unrestricted use, distribution, and reproduction in any medium, provided the original work is properly cited.
The paper presents the pressed joint technology using forming process with or without additional fastener. The capabilities for increasing the load-carrying ability of mechanical joints by applying special rivets and dies were presented. The experimental research focused on joining steel sheet metal made of different materials. The joint forming was performed with the solid round die and rectangular split die for riveted joint forming. The load-carrying ability of joints was evaluated by measuring the maximum load force in the shearing test in the tensile testing machine. The effect of joint forming process on joined material strain was compared by measuring the microhardness of the joints.
The assembly process development is driven by the automotive industry, especially by companies manufacturing car body elements. These companies are involved in developing and implementing new solutions which are more environmentally friendly.
The processes of plastic joining of sheet metal constructions are even more successful. These processes belong among “white manufacturing processes” . Unlike spot welding and welding, they do not emit dangerous vapors . Mechanical joining of sheet metals is commonly used to manufacture the controlled crush zones elements in cars [3, 4].
In most clinching joint cases, the static strength is lower than that for spot weld joints. The clinching joint strength can be increased by using higher forming force in order to achieve decreased bottom thickness “” of the cap part of the joint . Another method is using the modified forming with the rivet .
The tool geometry must be selected properly in order to provide optimum joint forming conditions while joining materials. The selection of optimal values is a problem mentioned in papers developed among the others by Oudjene et al. , Coppieters et al. , Roux and Bouchard .
The mechanical joint forming using the nonround split die with rivet is not a well-known problem.
The most up-to-date papers and the only ones on such joints forming capability are papers presented by Mucha, Kaščák, and Spišák . Another paper presenting the effectiveness of this joining method is the paper published by Mucha and Witkowski .
Thus the authors decided to present results of joint researches conducted by Technical University of Košice and Rzeszów University of Technology.
2. Clinch Riveting Process
The joining process in the ClinchRivet (CR) technology is similar to the self-pierce riveting (SPR) and clinching (CL). The lock consisting of joined sheet metals is created by the plastic deformation of a solid rivet . For CL technology, the lock is formed by the rigid punch along with relevant die. The upper sheet metal is perforated while pressing the rivet with the self-pierce riveting (SPR) technology. The sheet metals are locked by anchoring the rivet in the lower sheet metal.
Whereas, CR technology entails pressing the solid rivet and anchoring this rivet in the upper sheet metal. The upper sheet metal is anchored in the lower sheet material (Figure 1). In this way, the joint is created.
No fastener is required in the CL joint. SPR and CR require specially selected rivets: the tubular and solid one.
The material lock is created in CR joint, as this is also the case for CL joint. The measurable lock parameters are and (Figure 1(b)). The strength and the destruction mechanism of CR joint, similarly to CL joint, depend mainly on created lock size and the and ratio. The CR joint bottom thickness is a critical area for joint tightness. Figure 1(b) shows how to measure the joint bottom thickness.
3. Materials and Methods
The research experiments were conducted in order to determine the joining capability of different material by ClinchRivet riveting technology developed by Tox Pressotechnik .
The maximum joint load-carrying ability increase range and the joint structure hardness were observed. The joint quality evaluation was performed visually (externally) and internally by preparing metallographic microsections. For various joints, the lock parameters and were also measured. For selected variants of CR and CL joints the above mentioned lock parameters were compared.
The maximum strength of clinching joint was compared with ClinchRivet joint.
3.1. Sheets Material
The examined sheet metals were made of steel and aluminum alloy. The steel sheet plates of 0.8 mm thickness are used in car body elements in Volkswagen Group car assembly plant, Skoda Mlada Boleslav in Bratislava. For comparison purposes, the aluminum alloy 5754 sheet metal of the same thickness in H111 state, material number 3.3535, was used. Different mechanical properties enabled examining the joint forming capability by straining the rivet being pressed. The chemical composition and mechanical properties were presented in Tables 1 and 2.
3.2. The Rivet and Joint Forming Tools
Single rivet type of specified geometry (Figure 2) was used in joint forming; an average hardness of the steel rivet in five measurements was 357 HV0.1. The used rivet was made of material designated by the catalog number A5x5-2Al by TOX Pressotechnik. Main alloy additives in the chemical composition, besides carbon, are 0.35% Al and 1.5% Mn. The microstructure of the rivet material (zoom x500) is presented in Figure 3.
For all ClinchRivet rivet joining cases, we used the same die (Figure 4(a)). In the joining experiment, the Tox Pressotechnik die, catalog number TOX SKB 14.180.246182, was used.
The clinching joint (CL) was created with punch and die (Figure 4(b)) manufactured especially for thin sheet metal joining. These tools are used in the laboratory of Department of Technologies and Materials at the Technical University of Košice. The basic tool geometry was presented in Figure 4(c).
The CR rivet diameter was close to the diameter of die forming the CL joint.
Smaller die and punch diameters are dedicated in CL process for thin sheet metals. They result in a better lock in the overpress (cap part of the joint which is formed by the punch pressing the joined materials into the die) . Forming joints of sheet metal of different thickness are often accompanied by the material fracture. The tool geometry selection is especially important for thin sheet metals .
The die with CR rivet is more universal and forms high quality joints. The punch head with automatic rivet feeder was used while forming CR joints.
Joint forming was performed on the CMB frame press with an electric EMPK drive made by Tox Pressotechnik, maximum loading force of 100 kN. EMPK servo drive enables positioning the punch with 0.01 mm accuracy and measuring the joint forming force versus travel at maximum error of 0.5% force value. In all joining the rivet (CR) was pressed in order to achieve the flat surface of the upper sheet metal. The final punch position was set in order to achieve the distance between the die face and the punch face that equals the sum of sheet metal thicknesses. The distance value was defined in the control software of the press drive. This value was identical for all material combinations. Thus for different sheet materials different forming force was achieved.
CL joints were created for identical value of the bottom thickness. The value recommended by the tool manufacturers equals 25% of sum of joined sheet thicknesses. The same value was used in the experiment.
3.3. Joint Specimens and Combinations
The overlap joint specimens (Figure 5) were prepared for shearing test; 7 pieces for all arrangement. The force versus punch movement while forming was recorded.
The correct joint structure depends on many factors, including tool geometry, the strain hardening characteristics and material of sheet metal being joined, and rivet. The material flow while clinching process is limited to a small region around tools . The optimization of tool geometry for clinching process requires detailed knowledge on the material strain hardening characteristics. This issue was comprehensively presented by Coppieters et al. .
This paper focuses on effect of material type change on internal joint structure forming. Examined sheet plate arrangements are presented in Table 3.
CR joints were performed for all material variants from A to F and CL joints for variants A, C, and F.
3.4. Shear Tests and Microhardness
The shearing tests were performed on a universal tensile testing machine equipped with extensometer system and the sensor head for force measurements. The results were recorded by recording the joint shearing curve course in the static tension test of an overlap joint at 10 mm/min.
Sometimes the internal sheet metal defects cause the higher or lower joint strength. Higher differences of maximum joint shearing force were recorded in some cases during the experiment. Two most distinctive results were rejected, and subsequently the average value of 5 tests was calculated. To achieve the same test amount for each joining combination, the average of five results was accounted for.
The quality evaluation of clinching joints included metallographic and microhardness analyses. The 1N load was applied in measurements for about 15 s. The measurements were performed for specified locations on the joint cross-section (Figures 6(a) and 6(b)). Then the microsections were repolished and other measurements were performed. Three measurements were performed in each location. For tested materials, the starting material’s microhardness was measured.
In order to compare the rivet and sheet material strain hardening change, the microhardness measurement (Figure 6(c)) of the rivet in the sheet joint made of H220PD was performed.
4. Results and Discussion
The die with movable segments is required for CR joining (Figure 4(a)). Joining without a rivet requires no such a solution and the solid rigid die may be used (Figure 4(b)). Thus, the bulge of various shapes on the die contact side is achieved (Figure 7).
H220PD steel features the highest yield stress among all examined sheet materials. Large radial sheet metal plane transition into the bulge is visible right at the joint base (Figure 7(a)). On the other hand, in CL joint, the huge material breakdown may be observed on the bulge circumference (Figure 7(b)). Visible grooves show the difficult plastic material flow while pressing it into the die impression.
The bulge size in the die groove depends on the material type and tool geometry. This problem was clarified in several papers developed among the others by Mucha , Oudjene et al. , Jayasekara et al. , Lebaal et al. , Lee et al. , and Coppieters et al. . On the other hand, the ClinchRivet joint forming problem is rarely known.
Forming CR joints using DX51D + Z/RA-K 40/70 required the highest pressing force, whereas the highest joint shearing force was achieved for H220PD/H220PD (Figure 8).
The forming force generated by the riveting machine drive significantly deforms the riveting press frame . High strain of the joining device’s frame may lead to asymmetric joint forming.
Depending on sheet metal material type, for the same rivet different maximum shearing force and the shearing curve are achieved (Figure 9).
The maximum load-carrying ability of joints prepared with CR technology is several times higher comparing to joints prepared with CL technology (Figure 10) making the joint with rivet (CR) features a better forming, thus resulting in higher strength. Note the very high energy consumption of CR forming process comparing to CL technology without rivet. For sheet metal material layout “A,” the forming force was 22 kN, for layout “C” kN, and for layout “F” kN.
The typical feature of CR joint is that the overpress is stiffened by the pressed rivet, and for CL joint the inner part is empty (Figure 11). Thus a bit different joint destruction mechanism appears in shearing tests.
While shearing, the CL joint overpress separates by the necking material ductile failure (Figure 11, area “3”). The rest of sheet metal remains in the lower sheet material (Figure 12). This is one of the clinching joint’s destruction mechanisms .
The destruction mechanism of CR joint overpress is different comparing to CL joint. The separation is due to material ductile failure in area “1” (Figure 11) and due to complete pulling the rivet out of the lower sheet metal. The rivet remains in the upper sheet metal.
The upper sheet metal formed as a bulge by the rivet tears on its circumference (Figure 13). For H220PD, the fracture is visible in the bottom and on the circumference (Figure 13(a)). For remaining analyzed joints (made of DC06 and DX51D), the fracture occurred on the overpress circumference (Figures 13(b) and 13(c)).
Knowing the microhardness change, it is possible to forecast fracture sensitive areas. In the mechanical processes, the stress state, grain size, and material properties determined allowable deformations .
The values presented in Figure 14 were achieved by measuring the microhardness in specified locations on the metallographic microsections. The starting microhardness for corresponding sheet materials was indicated in brackets.
Different microhardness values were achieved both for CL and CR joints depending on the material type. The highest values were achieved for DX51D, and the lowest for DC06. This was related to mechanical properties and material’s strain hardening curve. Such a microhardness arrangement was observed for both CL and CR joints. For CR joint (Figure 14(b)), the microhardness differences between materials were higher than those for joints produced with CL technology (Figure 14(a)).
For CR joint, the microhardness values in measurement points “4” and “9” are higher than values for CL joint. Similar situation occurs in points “3” and “10.” As the segmented die has moving elements, it enables more intensive plastic material flow. While the material flows, the die segments move, and the material hardens more due to a plastic strain in previously mentioned areas of joint.
Whereas in the necking area of the upper sheet material for CR joint (in points “2” and “7”) the microhardness increase is lower than that for CL joint. For CR joint, the upper and lower sheets are slightly bent by the plastically flowing material of the joint bottom, while forming with the rigid die results in significant material extension, thus significantly increasing the material hardening and material hardness itself.
The initial structure of the rivet for CR technology was uniform and free of strain (Figure 3). No defects due to the rivet pressing were observed for each CR joint forming. The overpress bottom’s joined material thickness reduction occurred (Figure 15). The necking occured on the side surface, in a similar way to clinching joints . The largest gap between sheet metals occurred for DX51D (Figure 15(a)), and for remaining cases gaps were smaller (Figures 15(b) and 15(c)). The cylindrical surface thickness values were similar. The relevant differences were observed in the joint bottom, namely, at the deformed rivet edge.
The thicknesses of thinned upper and lower sheet DX51D were identical. Changing the material to DC06 resulted in excessive lower sheet thickness reduction, and the material continuity was maintained. While changing the sheet material to H220PD, the upper sheet metal thickness reduced and then the upper sheet fractured. This was due a different formability limit of joined materials.
For H220PD sheet material, the formability limit was achieved closely to the points. The microhardness values in points “4” and “9” (Figure 14(b)) and the sheet material continuity curve in the joint (Figure 15(c)) show that the formability limit for H220PD was achieved.
One of the highest CR joint forming forces was achieved for H220PD. For this material combination, the upper sheet metal fracture also occurred (Figure 15(c)-2). In this joint, the highest rivet’s microhardness increase occurred in its lower part locking the sheet material (Figures 6(c) and 16).
The material on the top of the rivet in its axis has no contact with the tool (tapered hole in the rivet). While pressing the rivet, firstly the rivet edges are upset, and then the material starts flowing in the lateral directions to the rivet axis. The microhardness increase was the highest in point “6” of this area.
The material on the rivet edges in the lower rivet part has a limited capability of plastic flow. The rivet edge is pressed into joined sheets. The lower part of the edge is bent outwards while pressing. The microhardness in point “4” of this area is lower than the value in point “6”.
Around the external rivet’s surface (points “1,” “2,” and “3”), the microhardness increase is not as high as an axial one, as a result of the initial shape. Around the external side and edge the rivet has to strain in extent that enables forming the lock without rivet fracture.
Depending on joined material arrangement, different lock forming occurs and the rivet deforms in different way (Figure 17). The lowest material lock was achieved for DX51D/RA-K 40/70 material arrangement (Figure 17(c) and Table 4). Changing the lower sheet from DX51D + Z to RA-K 40/70 (variants A and D) decreased by 57% and by 15% (Table 4). The rivet did not strain enough to deform the sheet metals. The rivet edges were upset, thus resulting in sheet metal thickness reduction in the lower part of the joint. The largest interlocking was achieved for material 5754, but both sheets material were thinned (Figure 17(d)). For sheets made of alloy 5754 parameter increased by 25%, and decreased by 34% comparing to joint made of DX51D + Z. For alloy 5754, the forming force was high, and the maximum load-carrying ability while shearing was quite low (Figure 8).
While comparing CL with CR for H220PD (both sheets), significant increase in parameter by 212% and parameter by 58% was observed (Table 4). For sheet metal arrangement according to variants “A” and “C”, the increased material locking was also observed. The highest improvement was achieved for variant “F”.
All the materials studied could be joined by clinching. With a few exceptions, this result was not expected at the outset of the study. The maximum shearing load depends heavily on the type of clinching method used (CL or CR) and varies significantly. For some material type arrangements, joining with rivet (CR) resulted in joint material separation.
The experimental CR joint forming analysis allowed researching the forming force depending on the sheet material type.
Depending on the joined material type, the rivet formed the joint, for which the maximum shearing force of joint overlapping was achieved.
For tested materials, the highest force was achieved for DX51D + Z/RA-K 40/70, and the lowest one was achieved for alloy 5754. For 5754, the highest difference between the forming force and the maximum shearing force was achieved. The high force value is due to a rivet material strain demand.
Applying the rivet for joint forming increases the lock size in sheet material () for DX51D + Z by 75% comparing to CL joint. However, forming the joint in this combination requires increasing the forming force by 290%.
Changing the joining method from CL to CR for material DC 06 increased the value by 123%. The force increased for this sheet material layout was 280%.
The best effect of lock increase in the joint was achieved while changing the joining method for H220PD material. The parameter increased by 150%. Increasing the lock size in this case of CR joint forming requires increasing the forming force by 283% compared to CL joint.
Clinching joints of 5 mm diameter feature much lower maximum joint strength compared to joint with an additional rivet. For DX51D + Z and DC06, the maximum joint shearing force increase was 150%. While for H220PD, the maximum joint shearing force increase was 316%.
CR joint forming pushes the unsafe material thinning area to the joint bottom. In CL joints, the necking locates in the center of the overpress height.
While joining different sheet metals, the critical thinning may occur, thus resulting in material layer fracture. The material discontinuities lower such a joint tightness. This may result in faster inner corrosion due to external factors.
Using the rivet in joint also changes the separation method. While shearing the CL joint, some part of the upper sheet metal remains in the lower sheet material. While shearing the CR joint, whole upper sheet metal remains on the rivet. The separation itself occurs by separating the sheet metals.
The paper was elaborated within the project “Application of progressive tool coatings for increasing the effectiveness and productivity of forming sheets made of modern materials” (APVV-0682-11).
- L. M. Alves, E. J. Dias, and P. A. F. Martins, “Joining sheet panels to thin-walled tubular profiles by tube end forming,” Journal of Cleaner Production, vol. 19, no. 6-7, pp. 712–719, 2011.
- J. Mucha, Ľ. Kaščák, and E. Spišák, “Joining the car-body sheets using clinching process with various thickness and mechanical property arrangements,” Archives of Civil and Mechanical Engineering, vol. 11, no. 1, pp. 135–148, 2011.
- B. Bartczak, D. Gierczycka-Zbrożek, Z. Gronostajski, S. Polak, and A. Tobota, “The use of thin-walled sections for energy absorbing components: a review,” Archives of Civil and Mechanical Engineering, vol. 10, no. 4, pp. 5–19, 2010.
- Z. Gronostajski and S. Polak, “Quasi-static and dynamic deformation of double-hat thin-walled elements of vehicle controlled body crushing zones joined by clinching,” Archives of Civil and Mechanical Engineering, vol. 8, no. 2, pp. 57–65, 2008.
- J. Mucha, “The analysis of lock forming mechanism in the clinching joint,” Materials and Design, vol. 32, no. 10, pp. 4943–4954, 2011.
- L. Kaščák, E. Spišák, and J. Mucha, “Evaluation of properties of joints made by clinching and self-piercing riveting methods,” Acta Metallurgica Slovaca, vol. 18, no. 4, pp. 172–180, 2012.
- R. Davies, R. Pedreschi, and B. P. Sinha, “The shear behaviour of press-joining in cold-formed steel structures,” Thin-Walled Structures, vol. 25, no. 3, pp. 153–170, 1996.
- R. F. Pedreschi, B. P. Sinha, and R. Davies, “Advanced connection techniques for cold-formed steel structures,” Journal of Structural Engineering, vol. 123, no. 2, pp. 138–144, 1997.
- R. F. Pedreschi and B. P. Sinha, “An experimental study of cold formed steel trusses using mechanical clinching,” Construction and Building Materials, vol. 22, no. 5, pp. 921–931, 2008.
- J. Mucha and W. Witkowski, “The experimental analysis of the double joint type change effect on the joint destruction process in uniaxial shearing test,” Thin-Walled Structures, vol. 66, pp. 39–49, 2013.
- M. Oudjene, L. Ben-Ayed, A. Delamézière, and J.-L. Batoz, “Shape optimization of clinching tools using the response surface methodology with Moving least-square approximation,” Journal of Materials Processing Technology, vol. 209, no. 1, pp. 289–296, 2009.
- S. Coppieters, P. Lava, S. Baes, H. Sol, P. Van Houtte, and D. Debruyne, “Analytical method to predict the pull-out strength of clinched connections,” Thin-Walled Structures, vol. 52, pp. 42–52, 2012.
- E. Roux and P. O. Bouchard, “Kriging metamodel global optimization of clinching joining processes accounting for ductile damage,” Journal of Materials Processing Technology, vol. 213, no. 7, pp. 1038–1047, 2013.
- F. Lambiase, “Influence of process parameters in mechanical clinching with extensible dies,” The International Journal of Advanced Manufacturing Technology, vol. 66, no. 9–12, pp. 2123–2131, 2013.
- F. Lambiase and A. Di Ilio, “Finite element analysis of material flow in mechanical clinching with extensible dies,” Journal of Materials Engineering and Performance, vol. 22, no. 6, pp. 1629–1636, 2013.
- S. Gao and L. Budde, “Mechanism of mechanical press joining,” International Journal of Machine Tools and Manufacture, vol. 34, no. 5, pp. 641–657, 1994.
- V. Jayasekara, K. H. Min, J. H. Noh et al., “Rigid-plastic and elastic-plastic finite element analysis on the clinching joint process of thin metal sheets,” Metals and Materials International, vol. 16, no. 2, pp. 339–347, 2010.
- N. Lebaal, M. Oudjene, and S. Roth, “The optimal design of sheet metal forming processes: application to the clinching of thin sheets,” International Journal of Computer Applications in Technology, vol. 43, no. 2, pp. 110–116, 2012.
- A. A. de Paula, M. T. P. Aguilar, A. E. M. Pertence, and P. R. Cetlin, “Finite element simulations of the clinch joining of metallic sheets,” Journal of Materials Processing Technology, vol. 182, no. 1–3, pp. 352–357, 2007.
- S. Coppieters, P. Lava, H. Sol, A. van Bael, P. van Houtte, and D. Debruyne, “Determination of the flow stress and contact friction of sheet metal in a multi-layered upsetting test,” Journal of Materials Processing Technology, vol. 210, no. 10, pp. 1290–1296, 2010.
- C.-J. Lee, J.-Y. Kim, S.-K. Lee, D.-C. Ko, and B.-M. Kim, “Design of mechanical clinching tools for joining of aluminium alloy sheets,” Materials and Design, vol. 31, no. 4, pp. 1854–1861, 2010.
- S. Coppieters, S. Cooreman, P. Lava, H. Sol, P. van Houtte, and D. Debruyne, “Reproducing the experimental pull-out and shear strength of clinched sheet metal connections using FEA,” International Journal of Material Forming, vol. 4, no. 4, pp. 429–440, 2011.
- T. Markowski, J. Mucha, and W. Witkowski, “FEM analysis of clinching joint machine’s c-frame rigidity,” Maintenance and Reliability, vol. 15, no. 1, pp. 51–57, 2013.
- F. Stachowicz, “Effects of microstructure on the mechanical properties and limit strains in uniaxial and biaxial stretching,” Journal of Mechanical Working Technology, vol. 19, no. 3, pp. 305–317, 1989.
- N. H. Hoang, O. S. Hopperstad, M. Langseth, and I. Westermann, “Failure of aluminium self-piercing rivets: an experimental and numerical study,” Materials and Design, vol. 49, pp. 323–335, 2013.
- W. Presz and R. Cacko, “Analysis of the influence of a rivet yield stress distribution on the micro-SPR joint—initial approach,” Archives of Civil and Mechanical Engineering, vol. 10, no. 4, pp. 69–75, 2010.